Glassy carbon is used nowadays for a variety of applications because of its mechanical strength, thermal stability and non-sticking adhesion properties. One application is glass molding that allows to realize high resolution diffractive optical elements on large areas and at affordable price appropriate for mass production. We study glassy carbon micro-structuring for future precision compression molding of low and high glass-transition temperature. For applications in optics the uniformity, surface roughness, edge definition and lateral resolution are very important parameters for a stamp and the final product. We study different methods of microstructuring of glassy carbon by etching and milling. Reactive ion etching with different protection layers such as photoresists, aluminium and titanium hard masks have been performed and will be compare with Ion beam etching. We comment on the quality of the structure definition and give process details as well as drawbacks for the different methods. In our fabrications we were able to realize optically flat diffractive structures with slope angles of 80° at typical feature sizes of 5 micron and 700 nm depth qualified for high precision glass molding.
Keywords: glassy carbon, reactive ion etching, ion beam etching, diffractive optical element, glass molding
1. INTRODUCTION Diffractive optics is making its way into industry through a large panel of applications, ranging from bio-technology via printing, material processing, sensing and optical metrology [1, 2]. Diffractive optical elements (DOEs) become key components for laser-based systems by controlling the shape of the beam . Compared to their refractive counterparts such as lenses, prisms or aspheres, diffractive optics can realize almost the same optical functions, while being much thinner and lighter .
Glass micro optical elements are currently mainly fabricated either by using direct precision machining process or by cleanroom micromachining technologies such as photolithography and etching [5-11]. For the economical manufacturing of high-precision glass optical elements, especially when it comes to mass production and high power applications, large-area replication-based technologies such as precision compression glass molding are promising alternatives [12-15]. Glass compression molding technology requires pressing a structured substrate into a glass substrate at a temperature close to the glass-transition temperature (Tg), which is higher than 400°C for low Tg glasses and becomes more than 1400°C for fused silica. The glass part then becomes the negative replica (reverse topography) of the mold.
Komori et al. and Yasui et al. have reviewed the characteristics of different mold materials for glass imprinting [16, 17]. Mold materials such as nickel, silicon or silicon dioxide, which are used for polymers injection molding, are not suitable for high Tg glass compression molding because of their poor heat stability and strong adhesion when releasing the glass part from the mold. However carbide-based hard alloys, such as tungsten carbide or silicon carbide, are commonly used to mold metals and glasses [14, 18-20].
Nanostructuring the mentioned alloys is quite difficult and leads to wasting expensive fabrication material. There are other interesting candidates, as for example graphene-coated silicon, copper-nickel alloy, nickel-phosphorus and chemical vapor-deposited diamond [16, 21-23].
Glassy carbon (glass-like carbon, vitreous carbon, GC) is especially interesting for compression glass molding of high Tg glasses, such as fused silica. The successful use of glassy carbon as a mold has been reported a couple of times during the last decade [24, 25]. Glassy carbon has interesting properties that are related to its fullerene-related structure and allows extreme operating temperature (up to 2000°C) . It is chemically inert and stable, and has a high hardness and a gas impermeability that leads to a low cohesion between glassy carbon and molding glasses [24, 27-29]. Glassy carbon can be polished and allows fabricating wafers of different sizes with high surface quality of λ/20 (over one inch length). The major drawback is that GC cannot easily be microstructured with conventional machines. But etching techniques and milling techniques known from microfabrication have been proven to be effective for depths in the order of micrometers. Different techniques for glassy carbon micro-structuration have already been tested. Kuhnke et al. have made a comparison between direct laser micromachining and reactive ion etching (RIE) , and Youn et al. and Takahashi et al. have investigated focused ion beam, nano/femtosecond-pulsed laser, excimer laser and dicing techniques [24, 30-32]. Dry etching of glassy carbon which results in a smooth surface quality has been highlighted by combining SF6/O2 during the RIE process [33, 34].
For the high-throughput application of glass molding to diffractive optics, despite the mentioned advances, it is necessary to investigate large-area-compatible process flows for microstructured GC with a high optical surface quality. Such an investigation is our main target in this manuscript. We describe different process flows based on photolithography and dry etching technologies. We first show the characterization results of the plasma etching of GC through a micro-structured photoresist (PR) layer at the surface of the substrate. We then compare these results with the etching of glassy carbon using either aluminium (Al) or titanium (Ti) hard masks and we describe the etching of GC using a broad-beam ion etcher (IBE).
2. EXPERIMENTAL PROCEDURE For this study a set of diffractive optical elements have been designed. It includes two-levels phase gratings which act as beam splitters and various test structures. We defined lateral feature sizes between 5 and 10 μm wide, with critical dimensions of about 2 μm. The active areas are between 5 and 18 mm in diameter. A picture of the quartz chrome (Cr) 5” photolithography mask used to pattern 4” glassy carbon wafers is given in Figure 1.
Different anisotropic etching techniques for glassy carbon structuring are investigated. The process flows are summarized in Figure 2. These processes are based on the use of 4” diameter double-side polished glassy carbon wafers with a thickness of 1 mm (substrates are AC-140 Glass Like Carbon Plate provided from Nisshinbo). The blank glassy carbon wafers delivered show a high surface quality with an average roughness RMSa < 5 nm.
Figure 1: 5” Quartz/Cr photolithography mask with the different diffractive structures
Proc. of SPIE Vol. 8974 89740Y-2
Figure 2: Overview of the four different investigated process flows (A to D). The processes are described in section 2. In section 3 a comparison between these processes with respect to their etching performance and resulting structure quality is made.
Proc. of SPIE Vol. 8974 89740Y-3
2.1 Glassy carbon reactive ion etching using a photoresist mask
The described process flow is based on the deposition and structuring of a single photoresist film which is to be used as a mask for reactive ion etching of glassy carbon (Figure 2: A). To enhance adhesion of photoresist on glassy carbon, hexamethyldislazane (HMDS) is used as a primer agent. A 2.8 μm positive photoresist film (MicroChemicals AZ 1518) is then deposited on the glassy carbon surface by spin coating (Convac), followed by a baking step on a hotplate for 1 min at 90°C. The photolithography process is done by illuminating the substrate during 2 sec with an intensity of 13 mW/cm2 through the photolithography mask in the mask aligner system (Süss Microtec MA8 GEN3). The substrate and the mask are in vacuum-contact mode during exposure to assure highest spatial resolution. The development is done during 45 sec with the remover AZ351B (MicroChemicals) in deionized water (DI). The concentration ratio between the remover and DI water is 1:4. The substrates are then rinsed and dried at 2400 rpm for 60 sec.
For the GC etching we used an inductively coupled plasma reactive ion etching (ICP-RIE) system (SPTS Advanced Plasma System). The glassy carbon wafers are conductive enough to be held on the electrostatic chuck without requiring a backside layer deposition; the measured helium-cooling leaks are about 50 mTorr/min when the substrate lies on the chuck. The electrodes frequency (RF) are 13.56 MHz, with a coil power of 950 W, a platen power of 100 W, a platen chiller at 20°C and a chamber pressure down to 37.5 mTorr. In order to avoid micro-masking effect, the used chemistry is O2/SF6. The gas flow rate was 40 and 10 sccm for O2 and SF6 respectively. The remaining photoresist at the substrate surface was then stripped by wet etching with Remover 1165 (Shipley Microposit) warmed at 70°C for 10 min, prior of rinsing and drying.
2.2 Glassy carbon plasma etching using an aluminium or a titanium hard mask
Aluminum and titanium were used as hard mask for reactive ion etching of glassy carbon (Figure 2: B and C). The fabrication steps are similar for both processes. Two thin titanium layers are sputtered before and after aluminium deposition to increase the adhesion between the aluminium hard mask and both substrate and photoresist. The metallic layer thickness is then 5nm Ti / 300nm Al / 5nm Ti for process flow B, and 500 nm Ti for process flow C. The deposition is made on the GC wafers using a sputtering system (Alliance-Concept DP 650). This step is followed by 140°C thermal dehydration for 10 min in an oven (Bita Yes III). A positive-type resist, AZ 1512 HS (MicroChemicals), was then spin-coated on the TiO2 surface layer (automatic coater and developer system EVG 150). This step was followed by 112°C baking for 1 min 30 sec on a hot plate, resulting in a film thickness of 1 μm. The resist film was then exposed through the photolithography mask in hard-contact mode with an intensity of 10 mW/cm2 for 1.5 sec (Süss MicroTec MA6/BA6). The wafers were developed to remove the exposed photoresist, and rinsed into DI water.
The metallic layers were etched in an ICP-RIE system (STS Multiplex). The etching parameters used for both Al and Ti etching processes were the same. The radio frequency power on the ICP electrodes was 13.56 MHz. The coil power inducing the plasma was at 800 W, and the platen power located below the substrate was at 150 W, for a chamber pressure of 3 mTorr and a platen chiller at 20°C. The used chemistry is Cl2/BCl3, with a gas flow rate of 10 sccm for both species. After hard mask layers etching, the substrates were rinsed into deionized water. This will avoid the hard mask corrosion through the creation of HCl that is obtained with the reaction between water vapor (coming from the cleanroom air when there is 45% or more humidity) and chlorine residues (that are remaining at the Al or Ti surface). The remaining PR film on the samples were then stripped on a wet bench containing two baths of Remover 1165 (Shipley Microposit) heated at 70°C, before being rinsed and dried.
For the GC etching we used another ICP-RIE system (SPTS Advanced Plasma System). The electrodes frequency was 13.56 MHz, with a coil power of 950 W and a platen power of 100 W. The chamber pressure is 37.5 mTorr. The substrate is cooled down with a platen chiller at 20°C. The used chemistry is O2/SF6, with a gas flow rate of 40 sccm, respectively 10 sccm. The substrates were then stripped by wet etching, prior of being rinsed and dried in a mixture of phosphoric, acetic and nitric acids warmed at 35°C for 10 min to remove Al, and hydrofluoric acid at room temperature for 5 min to remove Ti and TiO2 layers. To achieve a better Al stripping during wet etching after the RIE, it is advised to do an oxidization step using O2 plasma, which creates Al2O3. However as the use of O2 plasma without adding SF6 creates a rough surface for glassy carbon; this step has been put aside.
Proc. of SPIE Vol. 8974 89740Y-4
SO 100 SC 200
2.3 Glassy carbon ion beam etching using a photoresist mask
The process described here is based on the use of a microstructured photoresist mask deposited on a glassy carbon substrate that is etched by ion beam etching (Figure 2: D). The resist deposition and photolithography processes are nearly the same as previously described in subsection 2.1; however the photoresist film is 1060 nm thick here.
The etching process includes the use of an ion beam etcher system (Veeco NEXUS IBE-350) based on the ions bombardment of the glassy carbon substrate. To do so, the ions are extracted by current oscillations between parallel electrodes using a RF generator from argon gas located inside the discharged chamber. The Ar+ ions are then accelerated by a three-grid system (molybdenum apertures separated by a distance of a few millimeters), forming a collimated and invariant energy beam that is designed to etch large surface such as 4” wafer. The glassy carbon surface was etched with a tilt angle of 5° regarding the normal incidence of the ion beam while the substrate was rotating. The beam voltage was 500 V and its current 0.8 A. The electric current density was 1.2 mA/cm2.
3. RESULTS AND DISCUSSIONS 3.1 Glassy carbon reactive ion etching using a photoresist mask
The O2/SF6 process step to etch glassy carbon also etches the photoresist mask at the same time. The obtained GC etching rate is 110 nm/min, while the photoresist etching rate is 540 nm/min. The selectivity between GC and the PR mask is therefore only 1:5. This makes it very difficult to etch depth of a 1 micron into glassy carbon at very high resolution because the photoresist needs to be at least 5 micron high. Figure 3 shows the scanning electron microscopy (SEM) and white light interferometry picture (Veeco Wyko NT1100) of etching test results. Regarding the surface quality, we can see that there is no micro-masking effect with the used chemistry and etching parameters, and the structuring process provides high uniformity. The measured surface is smooth with a quite low roughness of RMSa < 20 nm. The surface is well stripped, although we have not used a PR ashing-step in an O2 plasma. However the edge quality is not satisfactory which is visible by the large bright lines. Such lines indicates that the edges are not sharp. The slope angle α is a parameter that measures the wall verticality. This angle α is defined as the tangent of the etching depth divided by the projected distance between the top and the bottom of the wall. For this process flow, the slope angle is α = 37°.
Figure 3: SEM image and white light interferometer image (VSI-mode) of photoresist micro-patterned glassy carbon. The structure height is 523 nm.
3.2 Glassy carbon plasma etching using an aluminum hard mask
The reactive ion etching process etched the 5nm Ti / 300nm Al / 5nm Ti layers from process flow B in about 80 sec. When the non-cover metallic layers are open, a strong contrasted color change of the dedicated wafer areas can be observed. This effect is due to the glassy carbon that is much less reflective than the aluminum layer. The etching stop-instant is determined by being 20 sec after the end of this color transition, in order to assure an uniform opening of the hard mask all over the substrate. The Al etching rate was 280 nm/min. The selectivity ratio between Al and the PR for
Proc. of SPIE Vol. 8974 89740Y-5
this process iglassy carbonof the structu
Figure 4low beca
The next stepThe etching ris then 1:0.4, 67°, overall vcontaminationsubstrates. Thre-deposited athere is no mwithout re-de
Figure 5. dots are dapplicatio
3.3 Glassy c
The Ti etchinopen the masafter the end
s 1:1.3. The ren. Thus the suures with the re
: a) A 325nm Pause the RIE did
p, based on therate is 230 nmmeaning that
very promisingn that happenhe reason is nand cannot be
Micrograph anddeposition of Alons.
ng process reqsk and to etchof the color ch
esist is then etrface quality oemaining phot
PR layer on 310d not attacked t
e use of O2/SFm/min and 100t aluminium isg parameters. ned during thnot fully exploe removed witg effect visibl
d SEM picture l compound of u
ma etching usi
quires the use h the 500 nm hange, as it ha
tched only sliof glassy carbtoresist on the
0 nm Al layer afthe GC surface.
F6 RIE, etches0 nm/min for Gs etched more Looking at th
he etching steored yet but itth conventione and roughn
of etched glassunknown nature
ng a titanium
of a rather thiTi layer tookas be done for
ghtly faster thbon is still sime metallic laye
fter STS RIE. R. b) A 310 nm th
s the glassy caGC and Al rethan two time
he structured sep can be seet is assumed t
nal methods. Inness is accepta
y carbon wafere during the etc
m hard mask
ick hard maskk about 140 ser Al hard mask
han the Al. Thmilar to blank sers and the har
Roughness of glhick Al layer af
arbon and the spectively. Thes faster thansurface in moren. Impuritiesthat non-volatn contrary to able (below R
r (depth = 460 nching process m
k of Ti of aboec and the etck previously.
he Cl2/BCl3 chsubstrates. Figrd mask in alu
lassy carbon in fter STS RIE an
Al hard maskhe related seleglassy carbonre details (as ss are visible tile particles othis unwanted
RMSa < 20 nm
nm) using Al asmaking the struc
ut 500 nm thiching stop instThe Ti etchin
hemistry does gure 4 illustrauminum.
the opened arend PR stripping
k with the follectivity betwen. The wall veshown in Figuall over the
of aluminum cd deposition, om) when mea
s hard mask. Thctures useless fo
ickness. The Rtant was deter
ng rate is abou
not react withates the quality
eas remains g.
lowing resultseen GC and Aerticality is α =ure 5), a heavyglassy carboncompound areone states thasured in areas
he small or optical
RIE process tormined 20 sec
ut 210 nm/min
s. Al = y n e
Proc. of SPIE Vol. 8974 89740Y-6
The particularesult is that athis oxide lay[35, 36]. The different etchstructures wit
Figure 6. the Ti sur
The etching sthe Ti surface(for GC deptremoving onlthan GC. Theto obtain a niis α = 79°. Tdemonstratesdepth is 506 n
Figure 7. boundarieetched sur
ty ratio is abo
arity with Ti ia thin layer ofyer is in the n effect of the
hing rate that th high vertica
a) High definitiface.
step with O2/Se, the TiO2/Tith of 506nm ly Ti, increasee stripping proce Ti removalThe parameter the high unifnm in this cas
a) Glassy carbes from the etchrface over a non
out 1:1 betwee
is its sensitivif titanium oxi
nm range at amtitanium oxidthe pure Ti) aality as shows
ion binary struc
SF6 species pri etching rate to 738nm, a
es the selectiviocess does nol. The glassy crs are overallformity procee.
bon edges are dhed TiO2 nativen-structured 1 m
en Ti and the
ity to oxygen ide is present mbient tempe
de layer is twoand the grainss in Figure 6.
ctures are show
rovides an etcis non-linear
and for relateity. TiO2 has t
ot requires stepcarbon surfacel very promis
ess for 50 µm
defined with 10e layer. b) Topmm2 surface. Th
that forms a when etching
erature (20°C)ofold. It leads s will alter the
wn after opening
ching rate of 5. The selectiv
ed TiO2/Ti dethen a smallerps such as sure quality then sing, as showlarge periods
00 nm width atology measuremhe RMSa is abo
The Cl2/BCl3 c
titanium oxid starts and it i, and the graito a non-lineae lateral resolu
g the Ti mask. b
512 nm/min fovity between Gepth of 123-2r etching rate trface activatioshows a rougn in Figure 7
s and over a 3
t a 506 nm depment (white lig
out 2 nm.
de layer (TiOis then slowlyin size can vaar etching chaution. The res
b) Grains of tita
or GC. Due toGC and TiO2/265nm). Etchithan GC, and on through O2ghness RMSa <7. The Figure3.5 mm of len
pth. The lateral ght interferomet
l does not rea
O2) when expoy removed. Thary between 2aracteristics (thsult are still h
anium oxide are
o the TiO2 lay/Ti vary from ing deeper inTi has a high
2 plasma befor< 5 nm. The we 8 b) (Brukength. The obta
resolution fits ter, PSI-mode)
act with glassy
osed to it. Thehe thickness o0 and 100 nmhe oxide has a
high quality T
e present at
yer diffused a1:0.2 to 1:0.5
nto GC, whileer etching ratere wet etching
wall verticalityr Dektak XT)
the grains of the GC
at 5 e e g y ) e
Proc. of SPIE Vol. 8974 89740Y-7
Figure 8. interferom
The Ti-mask titanium oxidtrue while etcIlluminating pattern.
Figure 9. projected
3.4 Glassy c
The GC ion bGC and the Pthick layer oRegarding throughness RMbeam millingmin, but this before doing
Glassy carbon meter measurem
process fulfilde layer is preching deeper the structures
a) Four-inches by the reflectio
carbon ion be
beam etching PR respectivelof photoresist e structure quMSa < 15 nmg process hardlayer was not the wet etch
structures with ment (VSI-mode
ls all necessarsent at the Ti than 740 nm s with a colli
glassy carbon on of a green las
eam etching u
through the mly. The selecti
is required. uality, after PR
m. We observedened a thin la
removed withhing step wou
50 µm period, e). b) Mechanic
ry requiremensurface, furthinto GC. Fig
imated laser b
wafer with diffser pointer (P =
using a photo
microstructureivity between High resolutiR stripping ane on Figure 1ayer of photorh such mean. uld be recomm
506nm depth acal profilometer
nts for the fabher investigatigure 9 a) showbeam results
fractive microst= 5 mW, λ = 53
ed PR mask sthe GC and th
ion and aspecnd at an etche0 that photorresist. A bath To have a wemended. How
and showing a hr measurement.
brication of diion are neededws the final suin the projec
tructures. The d3 nm).
hows an etchihe PR is 1: 2.5ct ratio are coed depth of 33esist residuesof solvent Sh
ell stripped surwever for glas
ffractive opticd to refine theurface of an etion of the re
depth is 738nm
ing rate of 125. In order to ompromised 31 nm, the sl are still pres
hipley 1165 atrface, an ashinssy carbon, th
y. a) White light
cal elements. e process. Thietched glassy elative design
m b) Beam splitt
2.3 and 30.4 netch 1 µm of for such thickope angle α isent at the surt 70°C has beeng-step in a Ohat implies ha
However as ais is especiallycarbon wafer
nm/min for thef GC, a 2.5 µmk mask layers 61°, and therface. The ionen used for 20
O2 plasma ovenaving a rough
a y r. n
e m r. e n 0 n h
Proc. of SPIE Vol. 8974 89740Y-8
surface (micro-masking effect). Piranha etching (sulfuric acid mixed with hydrogen peroxide, ratio: 4:1, for 10min at 40°C) has been performed and allowed us to remove part of the photoresist residues.
On the SEM pictures, we can see another drawback. The edges show sawtooth shapes instead of straight lines, and rounded corner instead of perpendicular corners. This kind of “wave effect” might be linked to the really low etching rate obtained. We were able to increase the beam intensity till a maximum etching rate of 24.3 and 48 nm/min for GC and PR respectively (at 700 V and 1.1 A). The selectivity between GC and PR is then about 1 : 2. Regarding the edges quality, the results are similar to the one observed in Figure 10. By comparison, using same etching beam parameters, hard materials such as TiW or AlTiC show low but in the same range etching rate, with 48 and 26 nm/min respectively, and a wave effect may also appears after etching such material. That effect could be avoid by modifying the design on the photolithography mask and then being able to compensate such unwanted shape. However that it a demanding work, especially for high-resolution diffractive optical gratings design.
The Table I provides a summary of the results related to the four investigated process flows (A to D), including etching rate, selectivity and structure quality.
Figure 10. SEM pictures of the GC structures after IBE and stripping. The structure shape shows an undesirable “wave effect”, especially in the angles. GC stripping after IBE is hard to perform, then a few PR remains at the surface. GC depth is 331 nm.
Table I. Results summary for the four investigated process flows (A to D).
Process flow A B C D
Description PR mask, GC RIE Al mask, GC RIE Ti mask, GC RIE PR mask, GC IBE
Surface quality High Low (residues exist) High Low (residues exist)
Proc. of SPIE Vol. 8974 89740Y-9
4. CONCLUSIONS We etched glassy carbon by reactive ion etching (process flow A, B and C) and by ion beam milling (process flow D) in section 2. Table 1 summarizes the results from section 3 related to etching rate, selectivity and structure quality. The photoresist-based processes (A and D) show an unfavorable etching ratio and lead to low edge definition. Aluminium hard masks cannot be used because of re-deposition of residues during the etching process of unknown constitution. Investigations are being done to clarify the cause of this problem. The third candidate to perform as a hard mask is titanium. Promising results could be obtained with this approach, as for example sharp edges or smooth surface. However titanium is not the preferred hard mask material because of its oxidation when exposed to air. Further characterizations are going to be done to understand this in more detail. Both aluminium and titanium have a smaller etching rate than glassy carbon which is preferential for high resolution and aspect ratio. The selectivity is 1:0.4 and 1:0.2-0.5 for Al and Ti respectively. This is much better than the 1:5 and 1:2.5 selectivity obtained between GC and photoresist using RIE and IBE. However an etching depth of 680 nm of GC still requires hard mask layers of over 300 nm Al or 500 nm Ti. The hard mask layer thicknesses are too large to use lift-off processes for hard mask structuring; etching is needed instead. This makes the process flow complicated and more expensive.
ACKNOWLEDGMENTS This research has been funded by the Commission for Technology and Innovation CTI under project number 12824.1 PFNM-NM. The authors thankfully acknowledge discussions with the partners from the ERANET-MNT-Guide4Diffractive project, and the technical support from the Center of Micro-nanotechnology (CMI) at EPFL.
REFERENCES  Gale, M. T., “Diffractive optics and micro-optics production technology in Europe,” OSA Trends in Optics and
Photonics (TOPS), Diffractive Optics and Micro-Optics, OSA Technical Digest 75, 18-20 (2002).  Kress, B. C. and Meyrueis, P., [Applied Digital Optics, from Micro-Optics to Nanophotonics], John Wiley &
Sons, Chichester, UK (2009).  Martinsson, H., Bengtsson, J., Ghisoni, M. and Larsson, A., “Monolithic Integration of Vertical-Cavity Surface-
Emitting Laser and Diffractive Optical Element for Advanced Beam Shaping,” IEEE Photonics Technol. Letters 11(5), 503-505 (1999).
 Herzig, H. P., [Micro-Optics: Elements, Systems and Applications], Taylor & Francis, London (1997).  Ronggui, S. and Righini, G. C., “Characterization of reactive ion etching of glass and its applications in
integrated optics,” Journal of Vacuum Science & Technology A 9, 2709 (1991).  Iliescu, C., Jing, Ji., Tay, E. H.F., Miao, J. and Sun, T., “Characterization of masking layers for deep wet
etching of glass in an improved HF/HCL solution,” Surface & Coatings Technol. 198, 314-318 (2005).  Wang, M. R. and Su, H., “Laser direct-write gray-level mask and one-step etching for diffractive microlens
fabrication,” Applied Optics 37, 7568-76 (1998).  Hirai, Y., Kanakugi, K., Yamaguchi, T., Yao, K., Kitagawa, S. and Tanaka, Y., “Fine pattern fabrication on
glass surface by imprint lithography,” Microelectron. Eng. 67-68, 237-244 (2003).  Gan, J., Wang, X., Zhou, M., Ngoi, B. And Zhong, Z., “Ultraprecision diamond turning of glass with ultrasonic
vibration,” J. Adv. Manuf. Technol. 21, 952-955 (2003).  Mertus, L. and Symmons, A., “Implications of diamond-turned vs diamond ground mold fabrication techniques
on precision-molded optics,” Proc. SPIE 8489 (2012).  Behrmann, G. P. and Duignan, M. T., “Excimer laser micromachining for rapid fabrication of diffractive optical
elements,” Applied Optics 36(20), 4666-4674 (2007).  Gale, M. T., “Replication techniques for diffractive optical elements,” Microelectronic Engineering 34, 321-339
(1997).  Gale, M. T., Gimkiewicz, C., Obi, S., Schnieper, M., Söchtig, J., Thiele, H. and Westenhöfer, S., “Replication
technology for optical microsystems,” Optics and Lasers in Engineering 43, 373-386 (2005).  Yi, A. Y. and Jain, A., “Compression molding of aspherical glass lenses – A combined experimental and
numerical analysis,” J. Am. Ceram. Soc. 88(3), 579-586 (2005).  Yi, A. Y., Chen, Y., Klocke, F., Pongs, G., Demmer, A., Grewell, A. And Benatar, A., “A high volume
precision compression molding process of glass diffractive optics by use of a micromachined fused silica wafer mold and low Tg optical glass,” J. Micromech. Microeng. 16(10), 2000-2005 (2006).
Proc. of SPIE Vol. 8974 89740Y-10
 Komori, M., Uchiyama, H., Takebe, H., Kusura, T., Kobayashi, K., Kubawahara, H. and Tsuchiya, T., “Micro/nanoimprinting of glass under high temperature using a CVD diamond mold,” J. Micromech. Microeng. 18, 065013 (2008).
 Yasui, M., Sugiyama, Y., Takahashi, M., Kaneko, S., Uegaki, J. I., Hirabayashi, Y., Sugimoto, K. I. and Maeda, R., “Fabrication of glassy carbon molds using hydrogen silsequioxane patterned by electron beam lithography as O2 dry etching mask,” Jpn J of Appl. Phys. 47, 5167-5170 (2008).
 Choi, W., Lee, J., Kim, W.-B., Min, B.-K., Kang, S. and Lee, S.-J.,“Design and fabrication of tungsten carbide mould with micro patterns imprinted by micro lithography,” J. Micromech. Microeng. 14, 1519-1525 (2004).
 Pang, S. W., Tamamura, T., Nakao, M., Ozawa, A. and Masuda, H., “Direct nano-printing on Al substrate using a SiC mold,” J. Vac. Sci. Technol. B 16, 1145-1149 (1998).
 Itoh, T., Tanaka, S., Li, J.-F., Watanabe, R. and Esashi M., “Silicon-carbide microfabrication by silicon lost molding for glass-press molds,” J. Microelectromech. Syst. 15(4), 859-863 (2006).
 He, P., Li, L., Yu, J., Huang, W., Yen, Y. C., Lee, L. J. and Yi, A. Y., “Graphene-coated Si mold for precision glass optics molding,” Optics Letters 38(14), 2625-2628 (2013).
 Pettersson, U. and Jacobson, S., “Tribological texturing of steel surfaces with a novel diamond embossing tool technique,” Tribol. Int. 39, 695-700 (2006).
 Hirai, Y., Yoshida, S., Takagi, n., Tanaka, Y., Yabe, H., Sasaki, K., Sumitani, H. and Yamamoto, K., “High aspect pattern fabrication by nano imprint lithography using fine diamond mold,” Jpn. J. Appl. Phys. 42, 3863-3866 (2003).
 Takahashi, M., Sugimoto, K. and Maeda, R., “Nanoimprint of glass materials with glassy carbon molds fabricated by focused-ion-beam etching,” Japan. J. Appl. Phys. 44, 5600-5605 (2005).
 Youn, S. W., Takahashi, M., Goto, H. and Maeda, R., “A study on fused ion beam milling of glassy carbon molds for the thermal imprinting of quartz and borosilicate glasses,” J. Micromech. Microeng. 16, 2576-2584 (2006).
 Harris, P. J. F., “Fullerene-related structure of commercial glassy carbons,” Philosophical Mag. 84:29, 3159-3167 (2004).
 Sasaki, T., Takahashi, M., Maeda, R., Tanaka, T., Maeno, T. and Yang, Z., “Microstructures formed on a low fluorescent glass using glassy carbon molding,” Proc. IEEE, Eng. in Medicine and Biology 27th Annual Conf., 7126-7128 (2005).
 Kuhnke, M., Lippert, Th., Ortelli, E., Scherer, G. G. and Wokaun, A., “Microstructuring of glassy carbon: comparison of laser machining and reactive ion etching,” Thin Solid Films 453-454, 36-41 (2004).
 Ito, H., Ito, K., Arai, M., Sugimoto, K. I., Matsukura, T. and Kogai, T., “Wettability between glass-like carbon and optical glasses,” J. Jpn. Soc. Precision Eng., 70(6), 807-811 (2004).
 Youn, S. W., Takahashi, M., Goto, H. and Maeda, R., “Microstructuring of glassy carbon mold for glass embossing – Comparison of focused ion beam, nano/femtosecond-pulsed laser and mechanical machining,” Microelectron. Eng. 83, 2482-2492 (2006).
 Youn, S. W., Takahashi, M., Goto, H. and Maeda, R., “Fabrication of micro-mold for glass embossing using focused ion beam, femto-second laser, excimer laser and dicing techniques,” J. Mater. Process. Technol. 187-188, 326-330 (2007).
 Takahashi, M., Murakoshi, Y., Maeda, R. and Hasegawa, K., “Large area micro hot embossing of pyrex glass with GC mold machined by dicing,” Microsyst. Technol. 13, 379-384 (2007).
 Youn, S. W., Ueno, A., Takahashi, M. and Maeda, R., “A process of glassy carbon etching without the micro masking effect for the fabrication of a mold with a high-quality surface,” J. Micromech. Microeng. 19, 125010 (2009).
 Mekaru, H., Okuyama, C., Ueno, A. and Takahashi, M., “Thermal imprinting on quartz fiber using glasslike carbon mold,” J. Vac. Sci. Technol. B 27(6), 2820-2824 (2009).
 Ting, C.-C. and Chen, S.-Y., “Structural evolution and optical properties of TiO2 thin films prepared by thermal oxidation of sputtered Ti films,” J. Appl. Phys. 88(8), 4628-4633 (2000).
 Fracassi, F. and Agostino, R. “Chemistry of titanium dry etching in fluorinated and chlorinated gases,” Pure & Appl. Chem. 64(5), 703-707 (1992).
Proc. of SPIE Vol. 8974 89740Y-11